#------------------------------------------------------------------------------
#$Date: 2016-02-18 17:37:37 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176729 $
#$URL: svn://www.crystallography.net/cod/cif/1/51/70/1517067.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1517067
loop_
_publ_author_name
'Xiu-Li Wang'
'Jing-Jing Cao'
'Guo-Cheng Liu'
'Hong-Yan Lin'
'Ai-Xiang Tian'
_publ_section_title
;
 Ligands directed versatile cadmium-bis(triazole) metal-organic fragments
 to generate three new two dimensional complexes based on polymolybdenum
 phosphate
;
_journal_name_full
;
Inorganica Chimica Acta
;
_journal_page_first              6
_journal_page_last               11
_journal_volume                  402
_journal_year                    2013
_chemical_formula_sum            'C14 H28 Cd3 Mo6 N12 O36 P4'
_chemical_formula_weight         1977.23
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                109.839(5)
_cell_angle_beta                 106.925(5)
_cell_angle_gamma                96.214(5)
_cell_formula_units_Z            2
_cell_length_a                   12.686(5)
_cell_length_b                   14.444(5)
_cell_length_c                   14.594(5)
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.15
_cell_measurement_theta_min      2.13
_cell_volume                     2341.9(15)
_computing_cell_refinement       'SMART (Bruker, 2001)'
_computing_data_collection       'SMART (Bruker, 2001)'
_computing_data_reduction        'SAINT+ (Bruker, 1999)'
_computing_molecular_graphics    'PLATON (Spek, 2003)'
_computing_publication_material  'SHELXTL (1998)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.986
_diffrn_measured_fraction_theta_max 0.986
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0176
_diffrn_reflns_av_sigmaI/netI    0.0360
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            11803
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.54
_exptl_absorpt_coefficient_mu    3.140
_exptl_absorpt_correction_T_max  0.864
_exptl_absorpt_correction_T_min  0.815
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            ORANGE
_exptl_crystal_density_diffrn    2.804
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       BLOCK
_exptl_crystal_F_000             1879
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.15
_refine_diff_density_max         1.280
_refine_diff_density_min         -1.179
_refine_diff_density_rms         0.188
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.124
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     679
_refine_ls_number_reflns         8138
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.124
_refine_ls_R_factor_all          0.0329
_refine_ls_R_factor_gt           0.0293
_refine_ls_shift/su_max          0.013
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0404P)²+3.4084P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0796
_refine_ls_wR_factor_ref         0.0814
_reflns_number_gt                7368
_reflns_number_total             8138
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ICA-2013-402-6-11-1.cif
_cod_data_source_block           compound_1
_cod_database_code               1517067
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
C1 C 1.1272(5) 0.3819(5) 0.1895(5) 0.0298(15) Uani 1 1 d .
H1 H 1.1471 0.3709 0.2509 0.036 Uiso 1 1 calc R
C2 C 1.0402(5) 0.3754(5) 0.0410(5) 0.0304(15) Uani 1 1 d .
H2 H 0.9839 0.3578 -0.0233 0.036 Uiso 1 1 calc R
C3 C 1.3088(5) 0.5033(5) 0.2267(6) 0.0391(17) Uani 1 1 d .
H3A H 1.3072 0.5721 0.2661 0.047 Uiso 1 1 calc R
H3B H 1.3466 0.5053 0.1781 0.047 Uiso 1 1 calc R
C4 C 1.3753(5) 0.4592(6) 0.3011(5) 0.0351(16) Uani 1 1 d .
H4A H 1.3663 0.4885 0.3680 0.042 Uiso 1 1 calc R
H4B H 1.3457 0.3867 0.2734 0.042 Uiso 1 1 calc R
C5 C 1.4997(5) 0.4811(6) 0.3151(5) 0.0427(19) Uani 1 1 d .
H5A H 1.5281 0.5535 0.3399 0.051 Uiso 1 1 calc R
H5B H 1.5414 0.4584 0.3674 0.051 Uiso 1 1 calc R
C6 C 1.5405(7) 0.4069(6) 0.0764(7) 0.053(2) Uani 1 1 d .
H6 H 1.5476 0.4162 0.0183 0.063 Uiso 1 1 calc R
C7 C 1.5261(5) 0.3352(5) 0.1763(5) 0.0291(14) Uani 1 1 d .
H7 H 1.5193 0.2876 0.2052 0.035 Uiso 1 1 calc R
C8 C 1.1348(5) 0.1283(5) -0.0929(5) 0.0282(14) Uani 1 1 d .
H8 H 1.0882 0.0912 -0.1616 0.034 Uiso 1 1 calc R
C9 C 1.2199(5) 0.1776(5) 0.0688(5) 0.0257(13) Uani 1 1 d .
H9 H 1.2416 0.1790 0.1360 0.031 Uiso 1 1 calc R
C10 C 1.2362(5) 0.2753(5) -0.1148(5) 0.0273(14) Uani 1 1 d .
H10A H 1.2913 0.2496 -0.1448 0.033 Uiso 1 1 calc R
H10B H 1.2704 0.3448 -0.0662 0.033 Uiso 1 1 calc R
C11 C 1.1331(5) 0.2728(5) -0.2000(5) 0.0305(15) Uani 1 1 d .
H11A H 1.0771 0.2969 -0.1705 0.037 Uiso 1 1 calc R
H11B H 1.1001 0.2037 -0.2500 0.037 Uiso 1 1 calc R
C12 C 1.1637(6) 0.3385(6) -0.2550(6) 0.0410(18) Uani 1 1 d .
H12A H 1.1933 0.4081 -0.2056 0.049 Uiso 1 1 calc R
H12B H 1.2225 0.3165 -0.2814 0.049 Uiso 1 1 calc R
C13 C 0.9292(4) 0.2857(5) -0.4850(4) 0.0196(12) Uani 1 1 d .
H13 H 0.8780 0.2482 -0.5519 0.024 Uiso 1 1 calc R
C14 C 1.0179(5) 0.4115(4) -0.3348(4) 0.0234(13) Uani 1 1 d .
H14 H 1.0389 0.4741 -0.2796 0.028 Uiso 1 1 calc R
N1 N 1.0290(4) 0.3384(4) 0.1116(4) 0.0281(12) Uani 1 1 d .
N2 N 1.1920(4) 0.4423(4) 0.1685(4) 0.0267(12) Uani 1 1 d .
N3 N 1.1384(4) 0.4390(4) 0.0712(4) 0.0298(12) Uani 1 1 d .
N4 N 1.5198(4) 0.4308(4) 0.2178(4) 0.0336(13) Uani 1 1 d .
N5 N 1.5271(7) 0.4782(5) 0.1523(6) 0.065(2) Uani 1 1 d .
N6 N 1.5433(4) 0.3181(4) 0.0882(4) 0.0265(12) Uani 1 1 d .
N7 N 1.1377(4) 0.1024(4) -0.0134(4) 0.0238(11) Uani 1 1 d .
N8 N 1.2087(4) 0.2154(4) -0.0591(4) 0.0227(11) Uani 1 1 d .
N9 N 1.2653(4) 0.2475(4) 0.0453(4) 0.0282(12) Uani 1 1 d .
N10 N 1.0665(4) 0.3328(4) -0.3400(4) 0.0286(12) Uani 1 1 d .
N11 N 1.0099(6) 0.2555(5) -0.4320(5) 0.058(2) Uani 1 1 d .
N12 N 0.9339(6) 0.3812(6) -0.4246(6) 0.061(2) Uani 1 1 d .
O1 O 1.0220(3) 0.1418(3) 0.1613(3) 0.0188(8) Uani 1 1 d .
O2 O 0.7462(3) 0.2720(3) 0.0076(3) 0.0198(8) Uani 1 1 d .
O3 O 0.7286(3) 0.1574(3) 0.1321(3) 0.0171(8) Uani 1 1 d .
O3W O 0.4280(3) 0.0831(3) 0.0038(3) 0.0299(10) Uani 1 1 d .
H3WA H 0.4160 0.0510 -0.0604 0.036 Uiso 1 1 d R
H3WB H 0.4469 0.0440 0.0349 0.036 Uiso 1 1 d R
O4 O 0.6913(3) 0.0297(3) 0.2060(3) 0.0155(8) Uani 1 1 d .
O4W O 0.8736(3) 0.0981(3) -0.0406(3) 0.0188(8) Uani 1 1 d .
H4WA H 0.8029 0.0893 -0.0517 0.023 Uiso 1 1 d R
H4WB H 0.8823 0.0821 -0.0991 0.023 Uiso 1 1 d R
O5 O 0.6960(3) 0.1058(3) 0.4152(3) 0.0130(7) Uani 1 1 d .
O6 O 0.4398(3) 0.2151(3) 0.2968(3) 0.0145(8) Uani 1 1 d .
O7 O 0.6411(3) 0.1973(3) 0.2709(3) 0.0167(8) Uani 1 1 d .
O8 O 0.6513(3) 0.3066(3) 0.4719(3) 0.0226(9) Uani 1 1 d .
O9 O 0.7772(3) -0.0752(3) 0.3311(3) 0.0216(9) Uani 1 1 d .
O10 O 0.8452(3) 0.1901(3) 0.3153(3) 0.0192(8) Uani 1 1 d .
O11 O 0.4439(3) 0.1495(3) -0.1657(3) 0.0133(7) Uani 1 1 d .
O12 O 0.4217(3) 0.0850(3) -0.3820(3) 0.0136(8) Uani 1 1 d .
O13 O 0.3163(3) -0.0762(3) -0.5957(3) 0.0133(8) Uani 1 1 d .
O14 O 0.4961(3) 0.1413(3) -0.5390(3) 0.0127(7) Uani 1 1 d .
O15 O 0.6322(3) 0.1298(3) -0.2230(3) 0.0121(7) Uani 1 1 d .
O16 O 0.6028(3) 0.2470(3) -0.3217(3) 0.0142(8) Uani 1 1 d .
O17 O 0.7939(3) 0.3131(3) -0.1341(3) 0.0175(8) Uani 1 1 d .
O18 O 0.6028(3) 0.3180(3) -0.1181(3) 0.0169(8) Uani 1 1 d .
O19 O 0.7765(3) 0.4485(3) 0.0167(3) 0.0228(9) Uani 1 1 d .
O20 O 0.8299(3) 0.2713(3) -0.3211(3) 0.0205(8) Uani 1 1 d .
O21 O 0.6527(3) 0.0401(3) -0.1005(3) 0.0146(8) Uani 1 1 d .
O22 O 0.4939(3) -0.0313(3) -0.2716(3) 0.0114(7) Uani 1 1 d .
O23 O 0.6914(3) -0.0333(3) -0.2712(3) 0.0126(7) Uani 1 1 d .
O24 O 0.3990(3) 0.2822(3) -0.2777(3) 0.0207(9) Uani 1 1 d .
O5W O 0.9196(4) 0.3694(3) 0.2676(4) 0.0415(12) Uani 1 1 d .
O28 O 1.0861(3) 0.0397(3) 0.2611(3) 0.0196(8) Uani 1 1 d .
O29 O 1.1348(3) -0.1430(3) 0.2060(3) 0.0157(8) Uani 1 1 d .
O30 O 1.2713(3) 0.1145(3) 0.4462(3) 0.0146(8) Uani 1 1 d .
O31 O 1.2189(3) 0.2015(3) 0.2972(3) 0.0161(8) Uani 1 1 d .
O32 O 1.3953(3) 0.3108(3) 0.4849(3) 0.0229(9) Uani 1 1 d .
O33 O 1.0946(3) -0.0588(3) 0.3996(3) 0.0224(9) Uani 1 1 d .
O34 O 1.0521(3) 0.2111(3) 0.3514(3) 0.0258(10) Uani 1 1 d .
P1 P 0.72838(11) 0.14414(10) 0.23213(10) 0.0120(3) Uani 1 1 d .
P2 P 0.72890(11) 0.33323(10) -0.05905(10) 0.0136(3) Uani 1 1 d .
P3 P 0.61901(10) 0.02535(10) -0.21454(10) 0.0098(3) Uani 1 1 d .
P4 P 1.09623(11) 0.14709(11) 0.26581(10) 0.0137(3) Uani 1 1 d .
Mo1 Mo 0.65421(4) -0.04126(3) 0.29791(3) 0.01110(10) Uani 1 1 d .
Mo2 Mo 0.57460(3) 0.19260(3) 0.38263(3) 0.01102(10) Uani 1 1 d .
Mo3 Mo 0.48808(4) 0.20865(3) -0.25466(3) 0.01128(11) Uani 1 1 d .
Mo4 Mo 0.75711(4) 0.20176(3) -0.27900(3) 0.01182(11) Uani 1 1 d .
Mo5 Mo 1.18256(4) -0.03158(3) 0.34131(3) 0.01248(11) Uani 1 1 d .
Mo6 Mo 1.37366(3) 0.19497(3) 0.39405(3) 0.01104(10) Uani 1 1 d .
Cd1 Cd 1.0000 0.0000 0.0000 0.02039(14) Uani 1 2 d S
Cd2 Cd 0.88685(3) 0.23028(3) 0.11650(3) 0.01627(10) Uani 1 1 d .
Cd3 Cd 0.58483(3) 0.17272(3) -0.00046(3) 0.01613(10) Uani 1 1 d .
Cd4 Cd 0.5000 0.0000 -0.5000 0.01229(12) Uani 1 2 d S
O2W O 0.1989(6) 0.4070(6) 0.4742(9) 0.169(6) Uani 1 1 d .
H2WA H 0.2046 0.3500 0.4789 0.203 Uiso 1 1 d R
H2WB H 0.2373 0.4168 0.4388 0.203 Uiso 1 1 d R
O1W O 0.2177(5) 0.5840(4) 0.6228(5) 0.0623(17) Uani 1 1 d .
H1WA H 0.2543 0.6452 0.6483 0.075 Uiso 1 1 d R
H1WB H 0.2265 0.5641 0.6725 0.075 Uiso 1 1 d R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N2 C1 N1 110.9(6) . .
N2 C1 H1 124.6 . .
N1 C1 H1 124.6 . .
N3 C2 N1 114.0(6) . .
N3 C2 H2 123.0 . .
N1 C2 H2 123.0 . .
N2 C3 C4 111.2(6) . .
N2 C3 H3A 109.4 . .
C4 C3 H3A 109.4 . .
N2 C3 H3B 109.4 . .
C4 C3 H3B 109.4 . .
H3A C3 H3B 108.0 . .
C5 C4 C3 110.4(6) . .
C5 C4 H4A 109.6 . .
C3 C4 H4A 109.6 . .
C5 C4 H4B 109.6 . .
C3 C4 H4B 109.6 . .
H4A C4 H4B 108.1 . .
N4 C5 C4 112.1(5) . .
N4 C5 H5A 109.2 . .
C4 C5 H5A 109.2 . .
N4 C5 H5B 109.2 . .
C4 C5 H5B 109.2 . .
H5A C5 H5B 107.9 . .
N5 C6 N6 115.0(7) . .
N5 C6 H6 122.5 . .
N6 C6 H6 122.5 . .
N6 C7 N4 109.7(6) . .
N6 C7 H7 125.2 . .
N4 C7 H7 125.2 . .
N7 C8 N8 109.5(5) . .
N7 C8 H8 125.3 . .
N8 C8 H8 125.3 . .
N9 C9 N7 114.0(5) . .
N9 C9 H9 123.0 . .
N7 C9 H9 123.0 . .
N8 C10 C11 112.0(5) . .
N8 C10 H10A 109.2 . .
C11 C10 H10A 109.2 . .
N8 C10 H10B 109.2 . .
C11 C10 H10B 109.2 . .
H10A C10 H10B 107.9 . .
C10 C11 C12 110.9(5) . .
C10 C11 H11A 109.5 . .
C12 C11 H11A 109.5 . .
C10 C11 H11B 109.5 . .
C12 C11 H11B 109.5 . .
H11A C11 H11B 108.1 . .
N10 C12 C11 111.3(5) . .
N10 C12 H12A 109.4 . .
C11 C12 H12A 109.4 . .
N10 C12 H12B 109.4 . .
C11 C12 H12B 109.4 . .
H12A C12 H12B 108.0 . .
N11 C13 N12 107.2(5) . .
N11 C13 H13 126.4 . .
N12 C13 H13 126.4 . .
N12 C14 N10 105.2(6) . .
N12 C14 H14 127.4 . .
N10 C14 H14 127.4 . .
C1 N1 C2 103.0(5) . .
C1 N1 Cd2 123.0(4) . .
C2 N1 Cd2 134.0(4) . .
C1 N2 N3 109.6(5) . .
C1 N2 C3 131.6(6) . .
N3 N2 C3 118.6(5) . .
C2 N3 N2 102.5(5) . .
C7 N4 N5 109.9(5) . .
C7 N4 C5 127.6(6) . .
N5 N4 C5 122.3(6) . .
C6 N5 N4 101.9(6) . .
C7 N6 C6 103.4(5) . .
C7 N6 Cd3 122.8(4) . 1_655
C6 N6 Cd3 133.5(4) . 1_655
C8 N7 C9 103.5(5) . .
C8 N7 Cd1 128.0(4) . .
C9 N7 Cd1 124.4(4) . .
C8 N8 N9 109.9(5) . .
C8 N8 C10 130.6(5) . .
N9 N8 C10 119.5(5) . .
C9 N9 N8 103.1(5) . .
N11 N10 C14 109.2(5) . .
N11 N10 C12 129.6(6) . .
C14 N10 C12 121.2(5) . .
C13 N11 N10 107.9(6) . .
C14 N12 C13 110.5(6) . .
P4 O1 Cd2 131.7(2) . .
P4 O1 Cd1 120.9(2) . .
Cd2 O1 Cd1 106.34(13) . .
P2 O2 Cd2 141.6(2) . .
P2 O2 Cd3 116.7(2) . .
Cd2 O2 Cd3 101.61(15) . .
P1 O3 Cd2 122.7(2) . .
P1 O3 Cd3 131.3(2) . .
Cd2 O3 Cd3 102.08(14) . .
Cd3 O3W H3WA 83.6 . .
Cd3 O3W H3WB 110.0 . .
H3WA O3W H3WB 107.7 . .
P1 O4 Mo1 129.1(2) . .
Cd1 O4W Cd2 108.51(14) . .
Cd1 O4W H4WA 130.5 . .
Cd2 O4W H4WA 83.3 . .
Cd1 O4W H4WB 88.0 . .
Cd2 O4W H4WB 147.1 . .
H4WA O4W H4WB 107.8 . .
Mo1 O5 Mo2 113.04(15) . .
Mo6 O6 Mo2 84.73(14) 1_455 .
P1 O7 Mo2 131.7(2) . .
Mo3 O11 Mo1 84.03(13) . 2_655
Mo3 O11 Cd3 118.91(16) . .
Mo1 O11 Cd3 140.30(18) 2_655 .
Mo3 O12 Mo1 83.20(13) . 2_655
Mo3 O12 Cd4 130.49(17) . .
Mo1 O12 Cd4 132.10(18) 2_655 .
Mo5 O13 Mo4 82.53(13) 1_454 2_654
Mo5 O13 Cd4 134.94(18) 1_454 .
Mo4 O13 Cd4 132.15(17) 2_654 .
Mo6 O14 Mo2 82.62(14) 1_454 1_554
Mo6 O14 Cd4 133.64(17) 1_454 .
Mo2 O14 Cd4 130.87(17) 1_554 .
P3 O15 Mo3 124.35(18) . .
P3 O15 Mo4 128.66(19) . .
Mo3 O15 Mo4 101.84(14) . .
Mo3 O16 Mo4 114.16(16) . .
P2 O17 Mo4 131.5(2) . .
P2 O18 Mo3 133.6(2) . .
P3 O21 Cd3 113.37(19) . .
P3 O22 Mo2 127.45(19) . 2_655
P3 O22 Mo1 125.6(2) . 2_655
Mo2 O22 Mo1 104.68(13) 2_655 2_655
P3 O23 Mo6 123.95(19) . 2_755
P3 O23 Mo5 126.4(2) . 2_755
Mo6 O23 Mo5 98.77(13) 2_755 2_755
P4 O28 Mo5 135.4(2) . .
Mo4 O29 Mo5 83.96(14) 2_755 .
Mo5 O30 Mo6 115.88(16) . .
P4 O31 Mo6 134.0(2) . .
O10 P1 O3 109.9(2) . .
O10 P1 O7 109.6(2) . .
O3 P1 O7 109.3(2) . .
O10 P1 O4 111.5(2) . .
O3 P1 O4 108.2(2) . .
O7 P1 O4 108.3(2) . .
O2 P2 O17 114.0(2) . .
O2 P2 O18 110.8(2) . .
O17 P2 O18 110.4(2) . .
O2 P2 O19 107.2(2) . .
O17 P2 O19 106.2(2) . .
O18 P2 O19 108.0(2) . .
O21 P3 O22 109.2(2) . .
O21 P3 O23 113.8(2) . .
O22 P3 O23 108.88(19) . .
O21 P3 O15 109.7(2) . .
O22 P3 O15 108.27(19) . .
O23 P3 O15 106.9(2) . .
O1 P4 O28 107.6(2) . .
O1 P4 O31 112.9(2) . .
O28 P4 O31 112.0(2) . .
O1 P4 O34 108.5(2) . .
O28 P4 O34 110.0(2) . .
O31 P4 O34 105.7(2) . .
O9 Mo1 O11 106.37(17) . 2_655
O9 Mo1 O12 101.43(17) . 2_655
O11 Mo1 O12 94.28(14) 2_655 2_655
O9 Mo1 O4 96.91(17) . .
O11 Mo1 O4 84.94(14) 2_655 .
O12 Mo1 O4 161.06(14) 2_655 .
O9 Mo1 O5 100.28(16) . .
O11 Mo1 O5 152.66(14) 2_655 .
O12 Mo1 O5 86.21(14) 2_655 .
O4 Mo1 O5 85.95(14) . .
O9 Mo1 O22 170.18(16) . 2_655
O11 Mo1 O22 82.82(13) 2_655 2_655
O12 Mo1 O22 80.94(14) 2_655 2_655
O4 Mo1 O22 80.20(13) . 2_655
O5 Mo1 O22 70.25(13) . 2_655
O9 Mo1 Mo3 100.41(14) . 2_655
O11 Mo1 Mo3 47.79(10) 2_655 2_655
O12 Mo1 Mo3 48.18(10) 2_655 2_655
O4 Mo1 Mo3 132.52(10) . 2_655
O5 Mo1 Mo3 132.75(10) . 2_655
O22 Mo1 Mo3 88.29(9) 2_655 2_655
O8 Mo2 O6 106.63(18) . .
O8 Mo2 O14 102.18(17) . 1_556
O6 Mo2 O14 94.63(14) . 1_556
O8 Mo2 O7 95.41(17) . .
O6 Mo2 O7 85.51(14) . .
O14 Mo2 O7 161.56(15) 1_556 .
O8 Mo2 O5 98.32(17) . .
O6 Mo2 O5 153.74(14) . .
O14 Mo2 O5 87.87(14) 1_556 .
O7 Mo2 O5 84.10(14) . .
O8 Mo2 O22 168.26(16) . 2_655
O6 Mo2 O22 84.40(14) . 2_655
O14 Mo2 O22 80.47(13) 1_556 2_655
O7 Mo2 O22 81.20(14) . 2_655
O5 Mo2 O22 70.22(12) . 2_655
O8 Mo2 Mo6 102.49(13) . 1_455
O6 Mo2 Mo6 47.54(10) . 1_455
O14 Mo2 Mo6 48.40(10) 1_556 1_455
O7 Mo2 Mo6 132.72(10) . 1_455
O5 Mo2 Mo6 134.46(10) . 1_455
O22 Mo2 Mo6 87.87(8) 2_655 1_455
O24 Mo3 O11 106.82(17) . .
O24 Mo3 O12 101.73(17) . .
O11 Mo3 O12 95.08(14) . .
O24 Mo3 O18 95.85(17) . .
O11 Mo3 O18 85.58(15) . .
O12 Mo3 O18 161.37(14) . .
O24 Mo3 O16 99.66(17) . .
O11 Mo3 O16 152.47(14) . .
O12 Mo3 O16 86.67(14) . .
O18 Mo3 O16 84.35(14) . .
O24 Mo3 O15 170.00(16) . .
O11 Mo3 O15 81.33(13) . .
O12 Mo3 O15 82.94(13) . .
O18 Mo3 O15 78.75(13) . .
O16 Mo3 O15 71.60(13) . .
O24 Mo3 Mo1 101.01(14) . 2_655
O11 Mo3 Mo1 48.18(10) . 2_655
O12 Mo3 Mo1 48.62(10) . 2_655
O18 Mo3 Mo1 133.57(11) . 2_655
O16 Mo3 Mo1 133.60(10) . 2_655
O15 Mo3 Mo1 88.73(9) . 2_655
O20 Mo4 O29 105.94(17) . 2_755
O20 Mo4 O13 102.36(17) . 2_654
O29 Mo4 O13 95.31(15) 2_755 2_654
O20 Mo4 O17 95.61(17) . .
O29 Mo4 O17 84.64(15) 2_755 .
O13 Mo4 O17 161.27(14) 2_654 .
O20 Mo4 O16 97.37(17) . .
O29 Mo4 O16 155.66(14) 2_755 .
O13 Mo4 O16 86.30(14) 2_654 .
O17 Mo4 O16 86.23(14) . .
O20 Mo4 O15 167.70(16) . .
O29 Mo4 O15 85.24(14) 2_755 .
O13 Mo4 O15 81.24(13) 2_654 .
O17 Mo4 O15 80.09(13) . .
O16 Mo4 O15 70.96(13) . .
O20 Mo4 Mo5 101.46(14) . 2_755
O29 Mo4 Mo5 48.19(10) 2_755 2_755
O13 Mo4 Mo5 48.64(10) 2_654 2_755
O17 Mo4 Mo5 132.56(11) . 2_755
O16 Mo4 Mo5 133.79(10) . 2_755
O15 Mo4 Mo5 89.78(9) . 2_755
O33 Mo5 O29 105.68(17) . .
O33 Mo5 O13 101.83(17) . 1_656
O29 Mo5 O13 95.15(15) . 1_656
O33 Mo5 O28 98.31(18) . .
O29 Mo5 O28 84.36(15) . .
O13 Mo5 O28 159.18(15) 1_656 .
O33 Mo5 O30 101.03(17) . .
O29 Mo5 O30 152.31(15) . .
O13 Mo5 O30 86.27(14) 1_656 .
O28 Mo5 O30 84.76(15) . .
O33 Mo5 O23 171.46(16) . 2_755
O29 Mo5 O23 81.47(14) . 2_755
O13 Mo5 O23 81.86(13) 1_656 2_755
O28 Mo5 O23 77.48(14) . 2_755
O30 Mo5 O23 71.35(13) . 2_755
O33 Mo5 Mo4 100.86(14) . 2_755
O29 Mo5 Mo4 47.85(11) . 2_755
O13 Mo5 Mo4 48.83(10) 1_656 2_755
O28 Mo5 Mo4 131.70(11) . 2_755
O30 Mo5 Mo4 133.14(10) . 2_755
O23 Mo5 Mo4 87.39(9) 2_755 2_755
O32 Mo6 O6 105.39(18) . 1_655
O32 Mo6 O14 102.54(17) . 1_656
O6 Mo6 O14 95.37(15) 1_655 1_656
O32 Mo6 O31 94.45(17) . .
O6 Mo6 O31 87.76(14) 1_655 .
O14 Mo6 O31 161.18(14) 1_656 .
O32 Mo6 O30 97.98(17) . .
O6 Mo6 O30 155.79(14) 1_655 .
O14 Mo6 O30 85.50(14) 1_656 .
O31 Mo6 O30 84.16(14) . .
O32 Mo6 O23 168.64(15) . 2_755
O6 Mo6 O23 82.71(14) 1_655 2_755
O14 Mo6 O23 84.30(13) 1_656 2_755
O31 Mo6 O23 77.68(13) . 2_755
O30 Mo6 O23 73.29(13) . 2_755
O32 Mo6 Mo2 101.86(13) . 1_655
O6 Mo6 Mo2 47.73(10) 1_655 1_655
O14 Mo6 Mo2 48.97(10) 1_656 1_655
O31 Mo6 Mo2 135.14(10) . 1_655
O30 Mo6 Mo2 133.15(10) . 1_655
O23 Mo6 Mo2 89.48(8) 2_755 1_655
N7 Cd1 N7 179.999(1) 2_755 .
N7 Cd1 O4W 90.02(16) 2_755 .
N7 Cd1 O4W 89.98(16) . .
N7 Cd1 O4W 89.98(16) 2_755 2_755
N7 Cd1 O4W 90.02(16) . 2_755
O4W Cd1 O4W 180.00(13) . 2_755
N7 Cd1 O1 94.09(15) 2_755 .
N7 Cd1 O1 85.91(15) . .
O4W Cd1 O1 71.70(12) . .
O4W Cd1 O1 108.31(12) 2_755 .
N7 Cd1 O1 85.91(15) 2_755 2_755
N7 Cd1 O1 94.09(15) . 2_755
O4W Cd1 O1 108.31(12) . 2_755
O4W Cd1 O1 71.69(12) 2_755 2_755
O1 Cd1 O1 180.0 . 2_755
N7 Cd1 Cd2 90.67(13) 2_755 .
N7 Cd1 Cd2 89.33(13) . .
O4W Cd1 Cd2 36.17(9) . .
O4W Cd1 Cd2 143.83(9) 2_755 .
O1 Cd1 Cd2 35.61(8) . .
O1 Cd1 Cd2 144.39(8) 2_755 .
N7 Cd1 Cd2 89.34(13) 2_755 2_755
N7 Cd1 Cd2 90.67(13) . 2_755
O4W Cd1 Cd2 143.83(9) . 2_755
O4W Cd1 Cd2 36.17(9) 2_755 2_755
O1 Cd1 Cd2 144.39(8) . 2_755
O1 Cd1 Cd2 35.61(8) 2_755 2_755
Cd2 Cd1 Cd2 180.0 . 2_755
N7 Cd1 H4WB 99.3 2_755 .
N7 Cd1 H4WB 80.7 . .
O4W Cd1 H4WB 20.2 . .
O4W Cd1 H4WB 159.8 2_755 .
O1 Cd1 H4WB 89.0 . .
O1 Cd1 H4WB 91.0 2_755 .
Cd2 Cd1 H4WB 54.6 . .
Cd2 Cd1 H4WB 125.4 2_755 .
O3 Cd2 N1 165.93(16) . .
O3 Cd2 O2 77.99(13) . .
N1 Cd2 O2 93.54(16) . .
O3 Cd2 O5W 90.76(15) . .
N1 Cd2 O5W 79.13(18) . .
O2 Cd2 O5W 97.60(17) . .
O3 Cd2 O1 105.73(14) . .
N1 Cd2 O1 86.51(17) . .
O2 Cd2 O1 156.88(13) . .
O5W Cd2 O1 105.09(16) . .
O3 Cd2 O4W 96.48(13) . .
N1 Cd2 O4W 93.68(16) . .
O2 Cd2 O4W 83.65(13) . .
O5W Cd2 O4W 172.75(15) . .
O1 Cd2 O4W 73.28(12) . .
O3 Cd2 Cd3 39.56(9) . .
N1 Cd2 Cd3 132.87(13) . .
O2 Cd2 Cd3 39.33(9) . .
O5W Cd2 Cd3 101.88(13) . .
O1 Cd2 Cd3 135.92(10) . .
O4W Cd2 Cd3 83.64(9) . .
O3 Cd2 Cd1 101.73(10) . .
N1 Cd2 Cd1 92.19(14) . .
O2 Cd2 Cd1 118.96(10) . .
O5W Cd2 Cd1 142.98(13) . .
O1 Cd2 Cd1 38.05(9) . .
O4W Cd2 Cd1 35.32(9) . .
Cd3 Cd2 Cd1 109.94(2) . .
O3 Cd2 H4WA 78.8 . .
N1 Cd2 H4WA 109.2 . .
O2 Cd2 H4WA 70.3 . .
O5W Cd2 H4WA 165.3 . .
O1 Cd2 H4WA 87.8 . .
O4W Cd2 H4WA 20.3 . .
Cd3 Cd2 H4WA 63.5 . .
Cd1 Cd2 H4WA 50.6 . .
N6 Cd3 O3W 89.19(17) 1_455 .
N6 Cd3 O2 87.44(16) 1_455 .
O3W Cd3 O2 175.74(14) . .
N6 Cd3 O3 101.11(16) 1_455 .
O3W Cd3 O3 101.60(14) . .
O2 Cd3 O3 76.52(13) . .
N6 Cd3 O21 169.06(15) 1_455 .
O3W Cd3 O21 101.40(14) . .
O2 Cd3 O21 82.10(13) . .
O3 Cd3 O21 79.62(12) . .
N6 Cd3 O11 93.38(15) 1_455 .
O3W Cd3 O11 78.56(14) . .
O2 Cd3 O11 104.23(12) . .
O3 Cd3 O11 165.52(12) . .
O21 Cd3 O11 86.13(12) . .
N6 Cd3 Cd2 101.72(13) 1_455 .
O3W Cd3 Cd2 139.63(11) . .
O2 Cd3 Cd2 39.06(9) . .
O3 Cd3 Cd2 38.36(9) . .
O21 Cd3 Cd2 71.97(8) . .
O11 Cd3 Cd2 138.10(8) . .
N6 Cd3 H3WA 103.5 1_455 .
O3W Cd3 H3WA 21.1 . .
O2 Cd3 H3WA 163.1 . .
O3 Cd3 H3WA 113.2 . .
O21 Cd3 H3WA 86.0 . .
O11 Cd3 H3WA 62.8 . .
Cd2 Cd3 H3WA 145.7 . .
O13 Cd4 O13 180.0 2_654 .
O13 Cd4 O12 81.81(12) 2_654 2_654
O13 Cd4 O12 98.19(12) . 2_654
O13 Cd4 O12 98.19(12) 2_654 .
O13 Cd4 O12 81.81(12) . .
O12 Cd4 O12 180.0 2_654 .
O13 Cd4 O14 84.71(13) 2_654 .
O13 Cd4 O14 95.29(12) . .
O12 Cd4 O14 97.69(12) 2_654 .
O12 Cd4 O14 82.31(12) . .
O13 Cd4 O14 95.29(12) 2_654 2_654
O13 Cd4 O14 84.71(13) . 2_654
O12 Cd4 O14 82.31(12) 2_654 2_654
O12 Cd4 O14 97.69(12) . 2_654
O14 Cd4 O14 180.0 . 2_654
H2WA O2W H2WB 107.8 . .
H1WA O1W H1WB 107.7 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 N2 1.306(8) .
C1 N1 1.326(8) .
C1 H1 0.9300 .
C2 N3 1.322(8) .
C2 N1 1.345(8) .
C2 H2 0.9300 .
C3 N2 1.473(7) .
C3 C4 1.534(9) .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
C4 C5 1.514(9) .
C4 H4A 0.9700 .
C4 H4B 0.9700 .
C5 N4 1.469(8) .
C5 H5A 0.9700 .
C5 H5B 0.9700 .
C6 N5 1.300(9) .
C6 N6 1.353(9) .
C6 H6 0.9300 .
C7 N6 1.311(8) .
C7 N4 1.329(8) .
C7 H7 0.9300 .
C8 N7 1.326(8) .
C8 N8 1.326(8) .
C8 H8 0.9300 .
C9 N9 1.301(8) .
C9 N7 1.360(7) .
C9 H9 0.9300 .
C10 N8 1.452(8) .
C10 C11 1.508(8) .
C10 H10A 0.9700 .
C10 H10B 0.9700 .
C11 C12 1.520(9) .
C11 H11A 0.9700 .
C11 H11B 0.9700 .
C12 N10 1.444(8) .
C12 H12A 0.9700 .
C12 H12B 0.9700 .
C13 N11 1.304(9) .
C13 N12 1.345(9) .
C13 H13 0.9300 .
C14 N12 1.320(9) .
C14 N10 1.342(8) .
C14 H14 0.9300 .
N1 Cd2 2.289(5) .
N2 N3 1.365(7) .
N4 N5 1.369(9) .
N6 Cd3 2.271(5) 1_655
N7 Cd1 2.262(5) .
N8 N9 1.365(7) .
N10 N11 1.347(8) .
O1 P4 1.513(4) .
O1 Cd2 2.321(4) .
O1 Cd1 2.457(4) .
O2 P2 1.509(4) .
O2 Cd2 2.304(4) .
O2 Cd3 2.317(4) .
O3 P1 1.536(4) .
O3 Cd2 2.273(4) .
O3 Cd3 2.333(4) .
O3W Cd3 2.282(4) .
O3W H3WA 0.8501 .
O3W H3WB 0.8500 .
O4 P1 1.549(4) .
O4 Mo1 2.066(4) .
O4W Cd1 2.332(4) .
O4W Cd2 2.381(4) .
O4W H4WA 0.8512 .
O4W H4WB 0.8479 .
O5 Mo1 2.118(3) .
O5 Mo2 2.136(4) .
O6 Mo6 1.930(4) 1_455
O6 Mo2 1.936(3) .
O7 P1 1.546(4) .
O7 Mo2 2.059(4) .
O8 Mo2 1.677(4) .
O9 Mo1 1.672(4) .
O10 P1 1.518(4) .
O11 Mo3 1.950(4) .
O11 Mo1 1.962(3) 2_655
O11 Cd3 2.436(3) .
O12 Mo3 1.966(3) .
O12 Mo1 1.979(3) 2_655
O12 Cd4 2.299(3) .
O13 Mo5 1.967(3) 1_454
O13 Mo4 1.972(3) 2_654
O13 Cd4 2.259(3) .
O14 Mo6 1.965(3) 1_454
O14 Mo2 1.982(4) 1_554
O14 Cd4 2.299(4) .
O15 P3 1.550(4) .
O15 Mo3 2.274(3) .
O15 Mo4 2.288(3) .
O16 Mo3 2.099(3) .
O16 Mo4 2.119(4) .
O17 P2 1.525(4) .
O17 Mo4 2.057(4) .
O18 P2 1.530(4) .
O18 Mo3 2.065(3) .
O19 P2 1.582(4) .
O20 Mo4 1.670(4) .
O21 P3 1.524(4) .
O21 Cd3 2.395(4) .
O22 P3 1.539(3) .
O22 Mo2 2.233(3) 2_655
O22 Mo1 2.249(3) 2_655
O23 P3 1.543(4) .
O23 Mo6 2.286(3) 2_755
O23 Mo5 2.401(3) 2_755
O24 Mo3 1.673(4) .
O5W Cd2 2.313(4) .
O28 P4 1.519(4) .
O28 Mo5 2.045(4) .
O29 Mo4 1.937(4) 2_755
O29 Mo5 1.948(4) .
O30 Mo5 2.086(4) .
O30 Mo6 2.113(4) .
O31 P4 1.525(4) .
O31 Mo6 2.092(3) .
O32 Mo6 1.678(4) .
O33 Mo5 1.676(4) .
O34 P4 1.569(4) .
Mo1 O11 1.962(3) 2_655
Mo1 O12 1.979(4) 2_655
Mo1 O22 2.249(3) 2_655
Mo1 Mo3 2.6189(10) 2_655
Mo2 O14 1.982(4) 1_556
Mo2 O22 2.233(3) 2_655
Mo2 Mo6 2.6057(12) 1_455
Mo3 Mo1 2.6188(10) 2_655
Mo4 O29 1.937(4) 2_755
Mo4 O13 1.972(3) 2_654
Mo4 Mo5 2.5981(10) 2_755
Mo5 O13 1.967(3) 1_656
Mo5 O23 2.401(3) 2_755
Mo5 Mo4 2.5981(10) 2_755
Mo6 O6 1.930(4) 1_655
Mo6 O14 1.965(3) 1_656
Mo6 O23 2.286(3) 2_755
Mo6 Mo2 2.6057(12) 1_655
Cd1 N7 2.262(5) 2_755
Cd1 O4W 2.332(4) 2_755
Cd1 O1 2.457(4) 2_755
Cd1 Cd2 3.8250(10) .
Cd1 Cd2 3.8251(11) 2_755
Cd1 H4WB 2.4530 .
Cd2 Cd3 3.5811(15) .
Cd2 H4WA 2.4335 .
Cd3 N6 2.271(5) 1_455
Cd3 H3WA 2.3439 .
Cd4 O13 2.259(3) 2_654
Cd4 O12 2.299(3) 2_654
Cd4 O14 2.299(4) 2_654
O2W H2WA 0.8590 .
O2W H2WB 0.8400 .
O1W H1WA 0.8501 .
O1W H1WB 0.8498 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
N2 C3 C4 C5 149.4(6) . .
C3 C4 C5 N4 -64.3(8) . .
N8 C10 C11 C12 178.4(6) . .
C10 C11 C12 N10 177.2(6) . .
N2 C1 N1 C2 1.2(7) . .
N2 C1 N1 Cd2 -178.0(4) . .
N3 C2 N1 C1 -0.4(8) . .
N3 C2 N1 Cd2 178.7(4) . .
N1 C1 N2 N3 -1.6(7) . .
N1 C1 N2 C3 -176.8(6) . .
C4 C3 N2 C1 24.4(10) . .
C4 C3 N2 N3 -150.4(6) . .
N1 C2 N3 N2 -0.5(7) . .
C1 N2 N3 C2 1.2(7) . .
C3 N2 N3 C2 177.2(6) . .
N6 C7 N4 N5 3.3(8) . .
N6 C7 N4 C5 179.0(6) . .
C4 C5 N4 C7 -81.0(9) . .
C4 C5 N4 N5 94.2(9) . .
N6 C6 N5 N4 -0.5(10) . .
C7 N4 N5 C6 -1.7(9) . .
C5 N4 N5 C6 -177.7(7) . .
N4 C7 N6 C6 -3.4(7) . .
N4 C7 N6 Cd3 171.0(4) . 1_655
N5 C6 N6 C7 2.4(10) . .
N5 C6 N6 Cd3 -171.1(6) . 1_655
N8 C8 N7 C9 -1.7(7) . .
N8 C8 N7 Cd1 156.1(4) . .
N9 C9 N7 C8 1.0(7) . .
N9 C9 N7 Cd1 -157.8(4) . .
N7 C8 N8 N9 1.9(7) . .
N7 C8 N8 C10 -179.2(6) . .
C11 C10 N8 C8 36.9(9) . .
C11 C10 N8 N9 -144.3(5) . .
N7 C9 N9 N8 0.1(7) . .
C8 N8 N9 C9 -1.2(7) . .
C10 N8 N9 C9 179.8(5) . .
N12 C14 N10 N11 -1.1(7) . .
N12 C14 N10 C12 179.3(6) . .
C11 C12 N10 N11 -70.1(9) . .
C11 C12 N10 C14 109.5(7) . .
N12 C13 N11 N10 -1.5(8) . .
C14 N10 N11 C13 1.6(7) . .
C12 N10 N11 C13 -178.7(6) . .
N10 C14 N12 C13 0.1(8) . .
N11 C13 N12 C14 0.9(8) . .
Cd2 O3 P1 O10 2.4(3) . .
Cd3 O3 P1 O10 -151.1(3) . .
Cd2 O3 P1 O7 122.6(2) . .
Cd3 O3 P1 O7 -30.8(3) . .
Cd2 O3 P1 O4 -119.6(2) . .
Cd3 O3 P1 O4 87.0(3) . .
Mo2 O7 P1 O10 -71.3(3) . .
Mo2 O7 P1 O3 168.3(3) . .
Mo2 O7 P1 O4 50.6(3) . .
Mo1 O4 P1 O10 67.1(3) . .
Mo1 O4 P1 O3 -171.9(2) . .
Mo1 O4 P1 O7 -53.6(3) . .
Cd2 O2 P2 O17 50.9(4) . .
Cd3 O2 P2 O17 -123.7(2) . .
Cd2 O2 P2 O18 176.1(3) . .
Cd3 O2 P2 O18 1.5(3) . .
Cd2 O2 P2 O19 -66.4(4) . .
Cd3 O2 P2 O19 119.1(2) . .
Mo4 O17 P2 O2 83.0(3) . .
Mo4 O17 P2 O18 -42.4(4) . .
Mo4 O17 P2 O19 -159.2(3) . .
Mo3 O18 P2 O2 -82.8(3) . .
Mo3 O18 P2 O17 44.5(4) . .
Mo3 O18 P2 O19 160.1(3) . .
Cd3 O21 P3 O22 -76.8(2) . .
Cd3 O21 P3 O23 161.36(18) . .
Cd3 O21 P3 O15 41.6(2) . .
Mo2 O22 P3 O21 -105.9(3) 2_655 .
Mo1 O22 P3 O21 93.9(3) 2_655 .
Mo2 O22 P3 O23 18.8(3) 2_655 .
Mo1 O22 P3 O23 -141.4(2) 2_655 .
Mo2 O22 P3 O15 134.7(2) 2_655 .
Mo1 O22 P3 O15 -25.5(3) 2_655 .
Mo6 O23 P3 O21 108.8(2) 2_755 .
Mo5 O23 P3 O21 -114.7(2) 2_755 .
Mo6 O23 P3 O22 -13.2(3) 2_755 .
Mo5 O23 P3 O22 123.3(2) 2_755 .
Mo6 O23 P3 O15 -130.0(2) 2_755 .
Mo5 O23 P3 O15 6.5(3) 2_755 .
Mo3 O15 P3 O21 -97.0(2) . .
Mo4 O15 P3 O21 113.1(2) . .
Mo3 O15 P3 O22 22.0(3) . .
Mo4 O15 P3 O22 -127.9(2) . .
Mo3 O15 P3 O23 139.2(2) . .
Mo4 O15 P3 O23 -10.7(3) . .
Cd2 O1 P4 O28 131.1(3) . .
Cd1 O1 P4 O28 -35.0(3) . .
Cd2 O1 P4 O31 -104.7(3) . .
Cd1 O1 P4 O31 89.1(3) . .
Cd2 O1 P4 O34 12.1(4) . .
Cd1 O1 P4 O34 -154.1(2) . .
Mo5 O28 P4 O1 158.4(3) . .
Mo5 O28 P4 O31 33.7(4) . .
Mo5 O28 P4 O34 -83.6(4) . .
Mo6 O31 P4 O1 -154.2(3) . .
Mo6 O31 P4 O28 -32.5(4) . .
Mo6 O31 P4 O34 87.3(3) . .
P1 O4 Mo1 O9 -101.4(3) . .
P1 O4 Mo1 O11 152.6(3) . 2_655
P1 O4 Mo1 O12 64.2(5) . 2_655
P1 O4 Mo1 O5 -1.6(3) . .
P1 O4 Mo1 O22 69.1(3) . 2_655
P1 O4 Mo1 Mo3 147.57(19) . 2_655
Mo2 O5 Mo1 O9 166.36(19) . .
Mo2 O5 Mo1 O11 -0.7(4) . 2_655
Mo2 O5 Mo1 O12 -92.69(18) . 2_655
Mo2 O5 Mo1 O4 70.06(17) . .
Mo2 O5 Mo1 O22 -10.97(14) . 2_655
Mo2 O5 Mo1 Mo3 -78.94(19) . 2_655
Mo6 O6 Mo2 O8 -91.87(17) 1_455 .
Mo6 O6 Mo2 O14 12.31(15) 1_455 1_556
Mo6 O6 Mo2 O7 173.81(15) 1_455 .
Mo6 O6 Mo2 O5 106.9(3) 1_455 .
Mo6 O6 Mo2 O22 92.24(13) 1_455 2_655
P1 O7 Mo2 O8 104.5(3) . .
P1 O7 Mo2 O6 -149.2(3) . .
P1 O7 Mo2 O14 -58.0(6) . 1_556
P1 O7 Mo2 O5 6.6(3) . .
P1 O7 Mo2 O22 -64.2(3) . 2_655
P1 O7 Mo2 Mo6 -143.0(2) . 1_455
Mo1 O5 Mo2 O8 -166.32(19) . .
Mo1 O5 Mo2 O6 -4.5(4) . .
Mo1 O5 Mo2 O14 91.68(18) . 1_556
Mo1 O5 Mo2 O7 -71.69(18) . .
Mo1 O5 Mo2 O22 11.05(14) . 2_655
Mo1 O5 Mo2 Mo6 76.95(19) . 1_455
Mo1 O11 Mo3 O24 89.84(17) 2_655 .
Cd3 O11 Mo3 O24 -124.48(19) . .
Mo1 O11 Mo3 O12 -14.05(14) 2_655 .
Cd3 O11 Mo3 O12 131.63(18) . .
Mo1 O11 Mo3 O18 -175.37(14) 2_655 .
Cd3 O11 Mo3 O18 -29.69(17) . .
Mo1 O11 Mo3 O16 -106.6(3) 2_655 .
Cd3 O11 Mo3 O16 39.1(4) . .
Mo1 O11 Mo3 O15 -96.10(13) 2_655 .
Cd3 O11 Mo3 O15 49.58(16) . .
Cd3 O11 Mo3 Mo1 145.7(2) . 2_655
Mo1 O12 Mo3 O24 -94.41(17) 2_655 .
Cd4 O12 Mo3 O24 123.8(2) . .
Mo1 O12 Mo3 O11 13.96(14) 2_655 .
Cd4 O12 Mo3 O11 -127.9(2) . .
Mo1 O12 Mo3 O18 105.2(4) 2_655 .
Cd4 O12 Mo3 O18 -36.6(6) . .
Mo1 O12 Mo3 O16 166.40(14) 2_655 .
Cd4 O12 Mo3 O16 24.6(2) . .
Mo1 O12 Mo3 O15 94.55(13) 2_655 .
Cd4 O12 Mo3 O15 -47.3(2) . .
Cd4 O12 Mo3 Mo1 -141.8(3) . 2_655
P2 O18 Mo3 O24 -156.2(3) . .
P2 O18 Mo3 O11 97.3(3) . .
P2 O18 Mo3 O12 4.5(7) . .
P2 O18 Mo3 O16 -57.0(3) . .
P2 O18 Mo3 O15 15.3(3) . .
P2 O18 Mo3 Mo1 92.6(3) . 2_655
Mo4 O16 Mo3 O24 164.98(18) . .
Mo4 O16 Mo3 O11 0.9(4) . .
Mo4 O16 Mo3 O12 -93.68(18) . .
Mo4 O16 Mo3 O18 69.98(17) . .
Mo4 O16 Mo3 O15 -10.01(14) . .
Mo4 O16 Mo3 Mo1 -79.58(18) . 2_655
P3 O15 Mo3 O24 -177.5(8) . .
Mo4 O15 Mo3 O24 -21.1(9) . .
P3 O15 Mo3 O11 37.3(2) . .
Mo4 O15 Mo3 O11 -166.28(15) . .
P3 O15 Mo3 O12 -58.9(2) . .
Mo4 O15 Mo3 O12 97.46(15) . .
P3 O15 Mo3 O18 124.5(3) . .
Mo4 O15 Mo3 O18 -79.10(15) . .
P3 O15 Mo3 O16 -147.8(3) . .
Mo4 O15 Mo3 O16 8.64(12) . .
P3 O15 Mo3 Mo1 -10.5(2) . 2_655
Mo4 O15 Mo3 Mo1 145.89(11) . 2_655
P2 O17 Mo4 O20 151.8(3) . .
P2 O17 Mo4 O29 -102.7(3) . 2_755
P2 O17 Mo4 O13 -12.0(7) . 2_654
P2 O17 Mo4 O16 54.7(3) . .
P2 O17 Mo4 O15 -16.6(3) . .
P2 O17 Mo4 Mo5 -97.1(3) . 2_755
Mo3 O16 Mo4 O20 -166.00(19) . .
Mo3 O16 Mo4 O29 -2.7(4) . 2_755
Mo3 O16 Mo4 O13 92.00(18) . 2_654
Mo3 O16 Mo4 O17 -70.81(18) . .
Mo3 O16 Mo4 O15 9.99(14) . .
Mo3 O16 Mo4 Mo5 80.33(18) . 2_755
P3 O15 Mo4 O20 165.4(6) . .
Mo3 O15 Mo4 O20 10.4(8) . .
P3 O15 Mo4 O29 -38.8(2) . 2_755
Mo3 O15 Mo4 O29 166.20(15) . 2_755
P3 O15 Mo4 O13 57.3(2) . 2_654
Mo3 O15 Mo4 O13 -97.67(15) . 2_654
P3 O15 Mo4 O17 -124.2(3) . .
Mo3 O15 Mo4 O17 80.83(15) . .
P3 O15 Mo4 O16 146.4(3) . .
Mo3 O15 Mo4 O16 -8.59(12) . .
P3 O15 Mo4 Mo5 9.2(2) . 2_755
Mo3 O15 Mo4 Mo5 -145.76(11) . 2_755
Mo4 O29 Mo5 O33 -90.56(18) 2_755 .
Mo4 O29 Mo5 O13 13.28(15) 2_755 1_656
Mo4 O29 Mo5 O28 172.37(15) 2_755 .
Mo4 O29 Mo5 O30 105.1(3) 2_755 .
Mo4 O29 Mo5 O23 94.23(13) 2_755 2_755
P4 O28 Mo5 O33 112.9(3) . .
P4 O28 Mo5 O29 -142.0(3) . .
P4 O28 Mo5 O13 -52.3(6) . 1_656
P4 O28 Mo5 O30 12.5(3) . .
P4 O28 Mo5 O23 -59.5(3) . 2_755
P4 O28 Mo5 Mo4 -134.4(3) . 2_755
Mo6 O30 Mo5 O33 -168.86(19) . .
Mo6 O30 Mo5 O29 -4.2(4) . .
Mo6 O30 Mo5 O13 89.80(18) . 1_656
Mo6 O30 Mo5 O28 -71.39(19) . .
Mo6 O30 Mo5 O23 7.14(15) . 2_755
Mo6 O30 Mo5 Mo4 74.7(2) . 2_755
P4 O31 Mo6 O32 -111.0(3) . .
P4 O31 Mo6 O6 143.8(3) . 1_655
P4 O31 Mo6 O14 43.6(6) . 1_656
P4 O31 Mo6 O30 -13.4(3) . .
P4 O31 Mo6 O23 60.8(3) . 2_755
P4 O31 Mo6 Mo2 137.3(2) . 1_655
Mo5 O30 Mo6 O32 165.13(19) . .
Mo5 O30 Mo6 O6 0.3(4) . 1_655
Mo5 O30 Mo6 O14 -92.80(18) . 1_656
Mo5 O30 Mo6 O31 71.45(18) . .
Mo5 O30 Mo6 O23 -7.42(15) . 2_755
Mo5 O30 Mo6 Mo2 -80.30(19) . 1_655
C8 N7 Cd1 N7 -86(4) . 2_755
C9 N7 Cd1 N7 67(4) . 2_755
C8 N7 Cd1 O4W -54.0(5) . .
C9 N7 Cd1 O4W 99.6(5) . .
C8 N7 Cd1 O4W 126.0(5) . 2_755
C9 N7 Cd1 O4W -80.4(5) . 2_755
C8 N7 Cd1 O1 -125.7(5) . .
C9 N7 Cd1 O1 27.9(5) . .
C8 N7 Cd1 O1 54.3(5) . 2_755
C9 N7 Cd1 O1 -152.1(5) . 2_755
C8 N7 Cd1 Cd2 -90.2(5) . .
C9 N7 Cd1 Cd2 63.4(5) . .
C8 N7 Cd1 Cd2 89.8(5) . 2_755
C9 N7 Cd1 Cd2 -116.6(5) . 2_755
Cd2 O4W Cd1 N7 91.10(18) . 2_755
Cd2 O4W Cd1 N7 -88.90(18) . .
Cd2 O4W Cd1 O4W -157(24) . 2_755
Cd2 O4W Cd1 O1 -3.20(13) . .
Cd2 O4W Cd1 O1 176.80(13) . 2_755
Cd2 O4W Cd1 Cd2 180.001(1) . 2_755
P4 O1 Cd1 N7 83.9(3) . 2_755
Cd2 O1 Cd1 N7 -85.43(18) . 2_755
P4 O1 Cd1 N7 -96.1(3) . .
Cd2 O1 Cd1 N7 94.57(18) . .
P4 O1 Cd1 O4W 172.5(3) . .
Cd2 O1 Cd1 O4W 3.24(14) . .
P4 O1 Cd1 O4W -7.5(3) . 2_755
Cd2 O1 Cd1 O4W -176.76(14) . 2_755
P4 O1 Cd1 O1 26(57) . 2_755
Cd2 O1 Cd1 O1 -143(57) . 2_755
P4 O1 Cd1 Cd2 169.3(4) . .
P4 O1 Cd1 Cd2 -10.7(4) . 2_755
Cd2 O1 Cd1 Cd2 180.0 . 2_755
P1 O3 Cd2 N1 -95.7(7) . .
Cd3 O3 Cd2 N1 64.2(7) . .
P1 O3 Cd2 O2 -149.6(3) . .
Cd3 O3 Cd2 O2 10.28(13) . .
P1 O3 Cd2 O5W -52.0(3) . .
Cd3 O3 Cd2 O5W 107.89(18) . .
P1 O3 Cd2 O1 53.9(3) . .
Cd3 O3 Cd2 O1 -146.20(13) . .
P1 O3 Cd2 O4W 128.3(2) . .
Cd3 O3 Cd2 O4W -71.79(15) . .
P1 O3 Cd2 Cd3 -159.9(3) . .
P1 O3 Cd2 Cd1 92.9(2) . .
Cd3 O3 Cd2 Cd1 -107.19(11) . .
C1 N1 Cd2 O3 98.6(8) . .
C2 N1 Cd2 O3 -80.4(9) . .
C1 N1 Cd2 O2 150.9(5) . .
C2 N1 Cd2 O2 -28.1(6) . .
C1 N1 Cd2 O5W 53.8(5) . .
C2 N1 Cd2 O5W -125.1(6) . .
C1 N1 Cd2 O1 -52.3(5) . .
C2 N1 Cd2 O1 128.8(6) . .
C1 N1 Cd2 O4W -125.2(5) . .
C2 N1 Cd2 O4W 55.8(6) . .
C1 N1 Cd2 Cd3 150.0(4) . .
C2 N1 Cd2 Cd3 -29.0(7) . .
C1 N1 Cd2 Cd1 -89.9(5) . .
C2 N1 Cd2 Cd1 91.1(6) . .
P2 O2 Cd2 O3 174.6(4) . .
Cd3 O2 Cd2 O3 -10.33(13) . .
P2 O2 Cd2 N1 6.0(4) . .
Cd3 O2 Cd2 N1 -178.98(17) . .
P2 O2 Cd2 O5W 85.5(4) . .
Cd3 O2 Cd2 O5W -99.49(16) . .
P2 O2 Cd2 O1 -83.4(5) . .
Cd3 O2 Cd2 O1 91.6(3) . .
P2 O2 Cd2 O4W -87.4(4) . .
Cd3 O2 Cd2 O4W 87.71(15) . .
P2 O2 Cd2 Cd3 -175.1(5) . .
P2 O2 Cd2 Cd1 -88.5(4) . .
Cd3 O2 Cd2 Cd1 86.55(13) . .
P4 O1 Cd2 O3 -78.6(3) . .
Cd1 O1 Cd2 O3 89.02(16) . .
P4 O1 Cd2 N1 94.3(3) . .
Cd1 O1 Cd2 N1 -98.05(18) . .
P4 O1 Cd2 O2 -174.9(3) . .
Cd1 O1 Cd2 O2 -7.2(4) . .
P4 O1 Cd2 O5W 16.5(3) . .
Cd1 O1 Cd2 O5W -175.80(15) . .
P4 O1 Cd2 O4W -170.8(3) . .
Cd1 O1 Cd2 O4W -3.15(13) . .
P4 O1 Cd2 Cd3 -109.3(3) . .
Cd1 O1 Cd2 Cd3 58.40(19) . .
P4 O1 Cd2 Cd1 -167.7(4) . .
Cd1 O4W Cd2 O3 -101.16(16) . .
Cd1 O4W Cd2 N1 88.59(19) . .
Cd1 O4W Cd2 O2 -178.25(17) . .
Cd1 O4W Cd2 O5W 81.4(13) . .
Cd1 O4W Cd2 O1 3.36(14) . .
Cd1 O4W Cd2 Cd3 -138.66(14) . .
N7 Cd1 Cd2 O3 -4.50(15) 2_755 .
N7 Cd1 Cd2 O3 175.50(15) . .
O4W Cd1 Cd2 O3 84.63(19) . .
O4W Cd1 Cd2 O3 -95.37(19) 2_755 .
O1 Cd1 Cd2 O3 -100.59(18) . .
O1 Cd1 Cd2 O3 79.41(18) 2_755 .
Cd2 Cd1 Cd2 O3 171(30) 2_755 .
N7 Cd1 Cd2 N1 177.60(17) 2_755 .
N7 Cd1 Cd2 N1 -2.40(17) . .
O4W Cd1 Cd2 N1 -93.3(2) . .
O4W Cd1 Cd2 N1 86.7(2) 2_755 .
O1 Cd1 Cd2 N1 81.5(2) . .
O1 Cd1 Cd2 N1 -98.5(2) 2_755 .
Cd2 Cd1 Cd2 N1 -7(30) 2_755 .
N7 Cd1 Cd2 O2 -87.14(16) 2_755 .
N7 Cd1 Cd2 O2 92.86(16) . .
O4W Cd1 Cd2 O2 1.99(19) . .
O4W Cd1 Cd2 O2 -178.01(19) 2_755 .
O1 Cd1 Cd2 O2 176.77(19) . .
O1 Cd1 Cd2 O2 -3.23(19) 2_755 .
Cd2 Cd1 Cd2 O2 89(30) 2_755 .
N7 Cd1 Cd2 O5W 102.8(2) 2_755 .
N7 Cd1 Cd2 O5W -77.2(2) . .
O4W Cd1 Cd2 O5W -168.0(3) . .
O4W Cd1 Cd2 O5W 12.0(3) 2_755 .
O1 Cd1 Cd2 O5W 6.7(2) . .
O1 Cd1 Cd2 O5W -173.3(2) 2_755 .
Cd2 Cd1 Cd2 O5W -81(30) 2_755 .
N7 Cd1 Cd2 O1 96.1(2) 2_755 .
N7 Cd1 Cd2 O1 -83.9(2) . .
O4W Cd1 Cd2 O1 -174.8(2) . .
O4W Cd1 Cd2 O1 5.2(2) 2_755 .
O1 Cd1 Cd2 O1 180.000(1) 2_755 .
Cd2 Cd1 Cd2 O1 -88(30) 2_755 .
N7 Cd1 Cd2 O4W -89.1(2) 2_755 .
N7 Cd1 Cd2 O4W 90.9(2) . .
O4W Cd1 Cd2 O4W 180.0 2_755 .
O1 Cd1 Cd2 O4W 174.8(2) . .
O1 Cd1 Cd2 O4W -5.2(2) 2_755 .
Cd2 Cd1 Cd2 O4W 87(30) 2_755 .
N7 Cd1 Cd2 Cd3 -44.83(12) 2_755 .
N7 Cd1 Cd2 Cd3 135.17(12) . .
O4W Cd1 Cd2 Cd3 44.29(16) . .
O4W Cd1 Cd2 Cd3 -135.71(16) 2_755 .
O1 Cd1 Cd2 Cd3 -140.93(16) . .
O1 Cd1 Cd2 Cd3 39.07(16) 2_755 .
Cd2 Cd1 Cd2 Cd3 131(30) 2_755 .
P2 O2 Cd3 N6 -71.2(3) . 1_455
Cd2 O2 Cd3 N6 112.18(18) . 1_455
P2 O2 Cd3 O3W -109(2) . .
Cd2 O2 Cd3 O3W 74(2) . .
P2 O2 Cd3 O3 -173.3(3) . .
Cd2 O2 Cd3 O3 10.12(13) . .
P2 O2 Cd3 O21 105.5(2) . .
Cd2 O2 Cd3 O21 -71.03(14) . .
P2 O2 Cd3 O11 21.6(3) . .
Cd2 O2 Cd3 O11 -154.98(13) . .
P2 O2 Cd3 Cd2 176.6(3) . .
P1 O3 Cd3 N6 62.5(3) . 1_455
Cd2 O3 Cd3 N6 -94.90(17) . 1_455
P1 O3 Cd3 O3W -29.0(3) . .
Cd2 O3 Cd3 O3W 173.64(15) . .
P1 O3 Cd3 O2 147.1(3) . .
Cd2 O3 Cd3 O2 -10.28(13) . .
P1 O3 Cd3 O21 -128.7(3) . .
Cd2 O3 Cd3 O21 73.99(14) . .
P1 O3 Cd3 O11 -118.2(5) . .
Cd2 O3 Cd3 O11 84.5(5) . .
P1 O3 Cd3 Cd2 157.4(4) . .
P3 O21 Cd3 N6 -66.2(9) . 1_455
P3 O21 Cd3 O3W 99.1(2) . .
P3 O21 Cd3 O2 -83.4(2) . .
P3 O21 Cd3 O3 -161.1(2) . .
P3 O21 Cd3 O11 21.6(2) . .
P3 O21 Cd3 Cd2 -122.2(2) . .
Mo3 O11 Cd3 N6 89.9(2) . 1_455
Mo1 O11 Cd3 N6 -151.4(3) 2_655 1_455
Mo3 O11 Cd3 O3W 178.4(2) . .
Mo1 O11 Cd3 O3W -62.9(3) 2_655 .
Mo3 O11 Cd3 O2 1.7(2) . .
Mo1 O11 Cd3 O2 120.3(3) 2_655 .
Mo3 O11 Cd3 O3 -89.4(5) . .
Mo1 O11 Cd3 O3 29.2(6) 2_655 .
Mo3 O11 Cd3 O21 -79.12(18) . .
Mo1 O11 Cd3 O21 39.5(3) 2_655 .
Mo3 O11 Cd3 Cd2 -21.8(2) . .
Mo1 O11 Cd3 Cd2 96.8(3) 2_655 .
O3 Cd2 Cd3 N6 93.2(2) . 1_455
N1 Cd2 Cd3 N6 -69.5(2) . 1_455
O2 Cd2 Cd3 N6 -70.9(2) . 1_455
O5W Cd2 Cd3 N6 16.64(18) . 1_455
O1 Cd2 Cd3 N6 143.49(19) . 1_455
O4W Cd2 Cd3 N6 -158.60(16) . 1_455
Cd1 Cd2 Cd3 N6 177.44(13) . 1_455
O3 Cd2 Cd3 O3W -9.6(2) . .
N1 Cd2 Cd3 O3W -172.3(2) . .
O2 Cd2 Cd3 O3W -173.7(2) . .
O5W Cd2 Cd3 O3W -86.2(2) . .
O1 Cd2 Cd3 O3W 40.7(2) . .
O4W Cd2 Cd3 O3W 98.60(19) . .
Cd1 Cd2 Cd3 O3W 74.64(17) . .
O3 Cd2 Cd3 O2 164.0(2) . .
N1 Cd2 Cd3 O2 1.4(2) . .
O5W Cd2 Cd3 O2 87.5(2) . .
O1 Cd2 Cd3 O2 -145.6(2) . .
O4W Cd2 Cd3 O2 -87.74(18) . .
Cd1 Cd2 Cd3 O2 -111.70(15) . .
N1 Cd2 Cd3 O3 -162.6(2) . .
O2 Cd2 Cd3 O3 -164.0(2) . .
O5W Cd2 Cd3 O3 -76.5(2) . .
O1 Cd2 Cd3 O3 50.3(2) . .
O4W Cd2 Cd3 O3 108.25(18) . .
Cd1 Cd2 Cd3 O3 84.28(15) . .
O3 Cd2 Cd3 O21 -96.09(18) . .
N1 Cd2 Cd3 O21 101.3(2) . .
O2 Cd2 Cd3 O21 99.89(18) . .
O5W Cd2 Cd3 O21 -172.60(15) . .
O1 Cd2 Cd3 O21 -45.76(16) . .
O4W Cd2 Cd3 O21 12.16(13) . .
Cd1 Cd2 Cd3 O21 -11.81(9) . .
O3 Cd2 Cd3 O11 -158.11(19) . .
N1 Cd2 Cd3 O11 39.3(2) . .
O2 Cd2 Cd3 O11 37.9(2) . .
O5W Cd2 Cd3 O11 125.38(18) . .
O1 Cd2 Cd3 O11 -107.78(18) . .
O4W Cd2 Cd3 O11 -49.86(16) . .
Cd1 Cd2 Cd3 O11 -73.83(13) . .
Mo5 O13 Cd4 O13 153(11) 1_454 2_654
Mo4 O13 Cd4 O13 -76(11) 2_654 2_654
Mo5 O13 Cd4 O12 -114.7(2) 1_454 2_654
Mo4 O13 Cd4 O12 16.2(3) 2_654 2_654
Mo5 O13 Cd4 O12 65.3(2) 1_454 .
Mo4 O13 Cd4 O12 -163.8(3) 2_654 .
Mo5 O13 Cd4 O14 -16.2(2) 1_454 .
Mo4 O13 Cd4 O14 114.8(2) 2_654 .
Mo5 O13 Cd4 O14 163.8(2) 1_454 2_654
Mo4 O13 Cd4 O14 -65.2(2) 2_654 2_654
Mo3 O12 Cd4 O13 14.1(2) . 2_654
Mo1 O12 Cd4 O13 -110.0(2) 2_655 2_654
Mo3 O12 Cd4 O13 -165.9(2) . .
Mo1 O12 Cd4 O13 70.0(2) 2_655 .
Mo3 O12 Cd4 O12 129(16) . 2_654
Mo1 O12 Cd4 O12 4(16) 2_655 2_654
Mo3 O12 Cd4 O14 -69.3(2) . .
Mo1 O12 Cd4 O14 166.5(2) 2_655 .
Mo3 O12 Cd4 O14 110.7(2) . 2_654
Mo1 O12 Cd4 O14 -13.5(2) 2_655 2_654
Mo6 O14 Cd4 O13 -168.5(2) 1_454 2_654
Mo2 O14 Cd4 O13 65.3(2) 1_554 2_654
Mo6 O14 Cd4 O13 11.5(2) 1_454 .
Mo2 O14 Cd4 O13 -114.7(2) 1_554 .
Mo6 O14 Cd4 O12 110.5(2) 1_454 2_654
Mo2 O14 Cd4 O12 -15.7(2) 1_554 2_654
Mo6 O14 Cd4 O12 -69.5(2) 1_454 .
Mo2 O14 Cd4 O12 164.3(2) 1_554 .
Mo6 O14 Cd4 O14 51(41) 1_454 2_654
Mo2 O14 Cd4 O14 -76(41) 1_554 2_654
